- Home
- Documents
*Ultrafast Probes for Dirac Materials ... Ultrafast Probes for Dirac Materials Quantum and Dirac...*

If you can't read please download the document

View

0Download

0

Embed Size (px)

Ultrafast Probes for Dirac Materials

Quantum and Dirac Materials Workshop March 8-11, 2015, Santa Fe, NM, USA

Center for Integrated Nanotechnologies Materials Physics and Applications Division

Los Alamos National Laboratory

Dmitry Yarotski

LANL Staff: Rohit Prasankumar, Antoinette Taylor, Abul Azad, Steve Gilbertson, George Rodriguez, Tomasz Durakiewicz, Aditya Mohite, Andrew Dattelbaum, Quanxi Jia, Stuart Trugman, Jian-xin Zhu

LANL Postdocs: Rolando Valdes Aguilar, Yaomin Dai, Keshav Dani, John Bowlan, Jingbo Qi, Jinho Lee, Georgi Dakovski

Brookhaven National Laboratory: Genda Gu, Ruidan Zhong

Rutgers University: Matthew Brahlek, Namrata Bansal, Seongshik Oh

Rice University: Sina Najmaei, Jun Lou, Pulickel M. Ajayan,

We gratefully acknowledge the support from the U.S. Department of Energy through the Center for Integrated Nanotechnologies, LANL LDRD Program, and the UC Office of the President under UC Lab Fees Research Program

Collaborators and Acknowledgements

Why Ultrafast Spectroscopy ? Ultrafast (10-100 fs) spectroscopy can resolve non-equilibrium dynamics

(quasiparticle, transport etc.) at the fundamental time and spatial scales of electronic and nuclear motion

Re tu

rn to

e qu

ili br

iu m

Time (ps)

Mn-O

Rini, Nature 449, 72 (2007) Kimel et al., Nature 435, 655 (2005)

Fausti, Science 2011

Manipulation of order parameters Photoinduced phase transitions New non-thermally accessible phases.

Ultrafast Coherent Order Manipulation

Vicario, Nature Phot. 2013

Graphene: The Slice that Started It All

Graphene: a basis for 0D buckyballs, 1D carbon nanotubes, and 3D graphite

Quasiparticles are described by relativistic Dirac equation – Dirac Material

Massless Dirac quasiparticles exhibit novel transport properties (high mobility, excellent conductivity)

after Castro Neto

Bonaccorso et al. Nat. Photonics 2010

Bae et al. Nat. Nanotech. 2010

Understanding the non-equilibrium behavior of photoexcited graphene is important for science and applications in detectors, solar cells and displays.

Quasiparticles in Graphene Linear dispersion near Dirac point gives for relativistic quasiparticles:

Measuring conductivity change after photoexcitation as function of N will indicate whether non-equilibrium quasiparticles are relativistic

Are photoexcited quasiparticles in graphene relativistic too?

Mak et al., Phys. Rev. Lett. (2008)

Two types of optical conductivity in graphene: Interband is constant in a wide

spectral range (flat 2.3% absorption) Intraband differs for linear and parabolic

bands

Measuring Relativistic Quasiparticles in Graphene

The change in conductivity, as measured in a visible pump-probe experiment, is dominated by the intraband component!

dopingIntrinsicraerexcitedPhotoraer )()( intintintint σσσσσ +−+=∆ −

We measure the photoinduced conductivity change:

1.55 eV pump, 1.77 eV probe experiments Fermi energy after photoexcitation = 700 meV (for N~3.1x1013/cm2) Decay dynamics are qualitatively identical for all photon energies (1.74-2.42 eV) Electron-electron thermalization within

Intraband contribution

dependence heN ,∝

Interband contribution

Reflectivity (or conductivity) change follows from

Our experiment reveals the relativistic nature of photoexcited Dirac quasiparticles in graphene

Hot Dirac Fermions in Graphene

K. M. Dani et al, Phys. Rev. B (2012)

Time-Resolved ARPES

M. Ferray, et al. J. Phys., 21 (1988); P.B. Corkum, PRL 71, 1994 (1993)

STATIC ARPES: probes electronic structure in both

E and k domains DYNAMIC ARPES: probes transient electronic

structure changes in both E and k domains

Fills excited states to reveal their structure

High Harmonic Generation – Extreme nonlinear frequency upconversion

Photoexcited Fermi-Dirac Distribution in Graphene

Is the Fermi-Dirac distribution of photoexcited carriers in graphene more like a metal (same μe and μh) or like a semiconductor (separate μe and μh)?

Do processes like Auger recombination influence the dynamics at early times?

Time-resolved photoemission experiments show that, in our samples, the photoexcited carriers retain separate F-D distributions for a few hundred femtoseconds

Recombination of Electronic States in Graphene

Ultrafast pump/probe experiment on CVD grown graphene 30 fs IR pump and sub-10 fs, 30-eV

probe via HHG measure tr-ARPES

A short-lived distribution of carriers and holes is formed after optical excitation.

Separate populations are: semi-conductor like (μ* ≠ 0) at early

delays metallic like (T* ≠ 0) at later times

S. Gilbertson et al,, JCP Letters (2012)

Topological Insulators

Moore et al., Nature 2010 Materials with exotic surface states Linear E-k dispersion TRS protection against scattering Locked spin-k relationship Majorana Fermions Spintronics, optoelectronics

Real materials are not ideal – dopants/defects result in significant bulk interference

THz spectroscopy provides the ability to separate the collective motion of charge carriers in bulk vs. surface states

* after A. Lanzara

Optical Pump Terahertz Probe

Low freq. spectra: Drude component: 1/τ ~ 1 THz Bulk phonon: ω0 ~ 1.9 THz Electron density consistent with nsurf ~ 1.5 x 1013 cm-2

Drude term is thickness independent Surface.

Phonon is not Bulk effect.

Terahertz Conductivity of Bi2Se3

Time-Resolved THz Spectroscopy Fix THz gate delay at maximum and scan pump-probe delay

Drude-Lorentz Model:

Well described by single carrier

type Carriers in 20 QL decay faster

Green: Drude (free electron). Purple: Phonon.

Photo-Induced Conductivity in Bi2Se3

Photo-Induced Drude Properties in 20 QL

Low Fluence: increase scat. rate -> increase T High Fluence: increase plasma freq. -> decrease T

Photo-Induced Phonon Frequency Shift in 20 QL

At high fluence, phonon shifts - similar to increase in temperature.

Highest lattice temperature ~ 200 K

Photo-Induced Drude Properties in 10 QL

Plasma frequency doesn’t change as much as in 20 QL sample.

Scattering rate does, so the sample becomes more transparent at higher fluence.

Physical Picture

Thin 10 QL films are similar to graphene: Surface electrons dominate, but

∆ωp is small Γsurf increases due to e-h

scattering and temperature rise (~200 K) due to e-ph relaxation

Thick 20 QL films: Surface response dominates at

low fluences High fluences result in large

number of bulk carriers => higher ∆ωp and Γbulk

Bulk electrons decay in ~5 ps Surface electrons decay in 20 ps

preserving high scattering rates

Hot surface carriers can be accessed independently from the bulk ones

using THz spectroscopy

Wang et al., Phys. Rev. Lett. 109, 127401 (2012) Sim et al., Phys. Rev. B 89, 165137 (2014)

Phonon-induced bulk-to-surface scattering is not effective below TD=180 K

R. Valdes Aguilar, Appl. Phys. Lett. (2015)

Topological Crystalline Insulators

Dirac Point

TI Time Reversal Symmetry

TCI Crystalline Symmetry

(001) surface

Metallic states on High Symmetry surfaces!

T and P-induced TPT

Pb0.77Sn0.23Se Dziawa et al. Nat. Mater. 11, 1023 (2012)

Gapped surface state Gapless surface state Linear dispersion

P-induced TPT in Pb1-xSnxSe Xi et al. PRL 113, 096401 (2014)

Topological Phase Transition in Pb1-xSnxSe

Topological Phase Transition in Pb1-xSnxTe

SnTe TCI

PbTe Trivial

Doping-driven Topological phase transition

Pb1-xSnxTe

Yan et al. PRL 112, 186801 (2014)

Can we use UOS to find the evidence for TPT with temperature and doping?

Xc = 0.4 at 5K

Preliminary Results and Future Directions

Doping-induced TPT at 5 K

Strong electron-phonon coupling in TI state – common to all TI

Investigate the effect of magnetic field using THz spectroscopy to probe conductivity of photoexcited carriers.

Apply circularly polarized pump to break TRS and study the dynamics of the k-spin locking process.

Xc ? Xc ?

Intervalley scattering

e-ph coupling

Coherent phonon

Temperature-induced TPT at x=0.4

Tc?

Temperature Dependence of Decay Amplitudes

Pb0.6Sn0.4Te

Slide Number 1 Slide Number 2 Slide Number 3 Slide Number 4 G